IMPACT: International Journal of Research in Engineering & Technology (IMPACT: IJRET) ISSN(E): 2321-8843; ISSN(P): 2347-4599 Vol. 3, Issue 8, Aug 2015, 31-40 ÂŠ Impact Journals

MACHINING PARAMETERS OPTIMIZATION IN END MILLING OF Ti6Al4V USING TAGUCHI METHOD AMAL T.S1, VIDYA V2 & ABRAHAM K VARUGHESE3 1

M.Tech Scholar, Department of Mechanical Engineering, Sree Buddha College of Engineering, University of Kerala, India

2

Assistant Professor, Department of Mechanical Engineering, Sree Buddha College of Engineering, University of Kerala, India 3

Scientist/Engineer SG, VSSC, Trivandrum, India

ABSTRACT Ti6Al4V has inevitable applications in aerospace industry where high surface finish is required. In this research the endmilling of annealed Ti6Al4V is performed using coated carbide inserts. The study in the effect of tool geometry has great importance in improving the quality of milled product.Cutting speed, feed rate, depth of cut and nose radius of milling cutter is selected as the input parameters. The responses observed are the surface roughness and cutting force. Taguchi method is employed for the design of experiments. L9 orthogonal array is selected for four factors and three levels by using MINITAB software. Each response is separately optimized by using signal to noise ratio analysis(S/N ratio analysis). ANOVA is employed to find out the percentage influence of input parameters on response. Optimum combination of machining parameters isobtained for surface roughness as well as for cutting force by using Taguchi based S/N ratio analysis.

KEYWORDS: Slot Milling, Nose Radius, Taguchi Method, Signal to Noise Ratio Analysis, Grey Relational Analysis, ANOVA

INTRODUCTION Titanium and its alloys are extensively used in aerospace because of their high specific strength, which is maintained at elevated temperature, their fracture resistant characteristics and their exceptional resistance to corrosion. They are being used increasingly in other industrial and commercial application such as petroleum refinery, nuclear reactors, surgical implants and marine application. They are also being used extensively for aerospace industry, mainly in airframe construction, where maximum ease of formability is desired.However,machining of titanium alloys involves expensive tooling cost at the expense of getting good surface roughness[1]. The main limiting factor in designing aircraft structures that involves dynamic loading is the fatigue property of the materials which is related to the surface

quality.

Therefore, the importance of surface integrity intitanium alloys milling process should be in

consideration. BalakrishnaRao et.al[2] have studied about facemilling of Ti6Al4V using simulations and experiments. This work concludes that the cutting speed has only a little contribution to cutting force and specific cutting energy.Khairi Yusuf and Y Nukman studiedflat end milling process that can produce a flat surface. Here, the rotation of cutter is perpendicular to the work piece of titanium alloys. The flat end milling with the multiple flute end mills, solid tool is used since the center cutting end teeth allows these end mills to drill into work piece to start a machining Impact Factor(JCC): 1.9586- This article can be downloaded from www.impactjournals.us

32

Amal T. S, Vidya V & Abraham K Varughese

operation[3].LohithakshaMMaiyaa, Dr.R.Ramanujam, and Dr.J.Jerald[4] have studied the effect of machining parameters on surface roughness and cutting force.It concludes that depth of cut has the most significant effect on cutting force followed by feed rate and cutting speed.The work also reveals that the most influencing parameter on surface roughness is feed rate followed by depth of cut and cutting speed.V Krishnaraja, S Samsudeensadham, R Sindhumathi, P Kuppan[5] have investigated high speed end milling of titanium alloy (Tiâ€“6% Alâ€“4% V) using carbide insert based end mill cutter. Effects of cutting forces during high speed machining of titanium alloys have got higher attention in selecting the optimal cutting conditions to improve the production and tool life. From this study it is found that depth of cut and feed rate have higher effect on cutting forces when compared to cutting speed.In this work,the machining parameters such as cutting speed,feedrate,depth of cut and nose radius are optimized for cutting force and surface roughness in end milling of Ti6Al4V using Signal to Noise ratio analysis. Coated carbideinserts are used in the milling operation [6].

NOMENCLATURE Vc- cutting speed in m/min f-feed rate in mm/min -axial depth of cut in mm -nose radius in mm OA-orthogonal array S/N-signal to noise ratio GRA-grey relational analysis Ra-average surface roughness F -force in x direction (in feed force) F -force in y direction (cross feed force) F -force in z direction (thrust force) F -resultant cutting force

-grey relational coefficient -distiguishing coefficient -grey relational grade DOF- Degree of freedom SS -Sum of squares MS-Variance of each factor %C -percentage contribution

Index Copernicus Value: 3.0 - Articles can be sent to editor@impactjournals.us

Machining Parameters Optimization in End Milling of Ti6al4v Using Taguchi Method

33

EXPERIMENTATION The response values required for the analysis is obtained by conducting nine slot milling operations.Slots of width 25mm were milled for a length of 84mm by considering the parameters such as cutting speed(m/min),feed rate(mm/min),depth of cut(mm) and nose radius(mm) and the measured output parameters are surface roughness and cutting force. The experiments are followed by Taguchi design and S/N ratio analysis. ANOVA is used to find out the percentage influence of input parameters on response.

WORKPIECE USED Ti6Al4V (Annealed) of size 90x84x10mm rectangular piece is used as workpiece. Similar six pieces are employed in the work for experimentation including confirmation experiments. Holes of diameter 8mm are drilled at the cornersof each work piece according to the top plate dimensions of dynamometer. Two experiments are performed (two slots) in each workpiece.The chemical composition and some mechanical properties of the workpiece material are given in the table 5.1 and 5.2 respectively. Figure 4.1 shows the actual image of the single workpiece. Figure 4.2 shows the dimensions of the workpiece used.

Figure 4.1: Work Piece Used

Figure 4.2: Drawing and Dimensions of Work Piece

PROPERTIES OF TI-6AL-4V Table 5.1: Chemical Composition Component Ti Al V Fe C

Percentage 89.55 6.40 3.89 0.16 0.002

Table 5.2: Mechanical Properties Hardness (HRC) Yield Strength Ultimate Tensile Strength Elongation Poissonâ€™s ratio Modulus of Elasticity Density Thermal Conductivity

36 900 MPa 950 MPa 14 % 0.342 113 GPa 4.43 g/m3 6.7 W/m-K

Impact Factor(JCC): 1.9586- This article can be downloaded from www.impactjournals.us

34

Amal T. S, Vidya V & Abraham K Varughese

CUTTING TOOL USED The cutting tool used is coated carbide inserts of grade WSP45S made by WALTER. The inserts used are of positive rhombic in shape and are shown in figure 6.1. Inserts of different nose radius are used for the studies (0.8 mm, 1.2 mm and 1.6 mm) which are ADMT 10 T3 08 R-F56,ADMT 10 T3 12 R-F56,ADMT 10 T3 16 R-F56.Each insert has two cutting edges. Six inserts of each type is used for the experiments.Total eighteen fresh inserts are used for the effective study of nose radius. The above mentioned three typesinsert show variations only in nose radius; all other features are same.The experiment was conducted on a DECKEL CNC 3 axis vertical milling machine and is shown in figure 6.3. The milling cutter of diameter 25mm is used for the slot milling operations.It holds three inserts. Figure 6.2 shows the milling cutter usedin the study. The specifications of milling cutter used is F 4042 R W 25 .025 Z03 10.

Figure 6:.1Inserts Used (Nose Radius: 0.8 Mm, 1.2 Mm And 1.6 Mm)

Figure 6.2: Millingcutter Used

Figure 6.3: CNC Milling Machine Used

DESIGN OF EXPERIMENTS USING TAGUCHI METHOD Design of experiments using the Taguchi method is employed to find out the optimum number of runs for the experiments with the combination of the parameters. Four input parameters and three levels are selected for the experiments. So, L9 orthogonal array with combination of input parameters and their levels are obtained using MINITAB software. The factors and levels of parameters are shown in table 7.1. Table 7.1 Factors and Levels Factors Cutting speed(m/min) Feed rate(mm/min) Depth of cut(mm) Nose radius(mm)

-1 24.7 60 1 0.8

0 31.4 120 1.5 1.2

1 39.3 180 2 1.6

Index Copernicus Value: 3.0 - Articles can be sent to editor@impactjournals.us

Machining Parameters Optimization in End Milling of Ti6al4v Using Taguchi Method

35

Total nine experiments are performed according to the L9 orthogonal array.

EXPERIMENT SET UP The KISTLER made tool dynamometer is fixed on the machine table.Work pieceis fixed over the tool dynamometer plate using M8 nuts.Tool dynamometer is connected to an amplifier through cables. Amplifier is connected to a computer using cables to record the cutting force data.Coolant applied during the milling operation is HOTCUT 795 H and is supplied in flood mode. The water soluble ratio of the coolant used is 1:9. The experiment setup including the work piece and tool setup, dynamometer and its accessory connections are shown in the figure 8.1 and 8.2.

Figure 8.1: Experiment Setup

Figure 8.2: Amplifier and Computer Used for Force Measurement

CUTTING FORCE AND SURFACE ROUGHNESS MEASUREMENT Cutting Force Measurement The force in Xdirection (in feed force), Ydirection (cross feed force) and Z direction ( thrust force) are measured using KISTLER made multi component tool dynamometer of type 9257B. The force obtained in each axis is averaged along the time domain between the times of engagement of cutter in the slot to the time of disengagement of the cutter at the end of the slot. The forces F (in feed force), F (cross feed force) and F (thrust force) are used to calculate F (resultant cutting force) by using the equation1[7]. F = âˆš F + F + F

(1)

Surface Roughness Measurement Surface roughness (Ra) is measured using Talysurf roughness tester. Ra in the starting, centre and ending points of each slot are measured and its average is taken as the surface roughness for the experiment.Surface roughness is measured for a sampling length of 4mm and a cut off length of 0.8mm.

Impact Factor(JCC): 1.9586- This article can be downloaded from www.impactjournals.us

36

Amal T. S, Vidya V & Abraham K Varughese

RESULTS AND ANALYSIS

Figure 10.1: Work Pieces after Slot Milling Operations Table 10.1 Experiment Results Run

Vc (M/Min)

F (Mm/Min)

Ap (Mm)

(Mm)

Ra (Îœm)

1

24.7

60

1

0.8

0.2318

432.6035

2

24.7

120

1.5

1.2

0.6121

528.9070

3

24.7

180

2

1.6

0.7733

713.5275

4

31.4

60

1.5

1.6

0.2185

487.6598

5

31.4

120

2

0.8

0.2825

500.7595

6

31.4

180

1

1.2

0.4130

551.6736

7

39.3

60

2

1.2

0.2713

544.0877

8

39.3

120

1

1.6

0.3957

490.0413

9

39.3

180

1.5

0.8

0.5874

522.8327

(N)

S/N RATIO ANALYSIS The S/N ratios are derived from the quadratic loss function and are expressed in a decibel scale (dB). Once all of the S/N ratios have been computed for each run of an experiment, Taguchi advocates a graphical approach to analyze the data. In the graphical approach, the S/N ratios and average responses are plotted for each factor against each of its levels.There are three standard types of S/N ratios depending on the desired performance response such as larger the better, nominal the better and smaller the better.Here,Surface roughness and cutting force are optimized using smaller the better relation[8]. The best condition is the one which maximize the appropriate S/N ratio. Table 11.1 shows the S/N ratios calculated for Ra and F using the equation 2. Smaller the better (for making the system response as small as possible): (

1 = âˆ’10 log & ' 2 % )*

Index Copernicus Value: 3.0 - Articles can be sent to editor@impactjournals.us

37

Machining Parameters Optimization in End Milling of Ti6al4v Using Taguchi Method

Table 11.1 S/N Ratios of Responses Experimen t 1 2 3 4 5 6 7 8 9

Ra (Îœm) 0.2318 0.6121 0.7733 0.2185 0.2825 0.4130 0.2713 0.3957 0.5874

S/N Ratio Of Ra (Db) 12.6906 4.2633 2.2250 13.2007 10.9550 7.670 11.2996 8.0456 4.6152

(N) 432.6035 528.9070 713.5275 487.6598 500.7595 551.6736 544.0877 490.0413 522.8327

S/N Ratio of (Db) -52.7218 -54.4675 -57.0682 -53.7623 -53.9925 -54.8336 -54.7133 -53.8046 -54.3672

Figure 11.1: Data Analysis Plot for S/N Ratio of Ra Figure 11.2: Data Analysis Plot for S/N Ratio of From the figure 11.1, the optimized parameters for minimum surface roughness are obtained. Optimized parameters for Ra are cutting speed 31.4m/min, feed rate 60mm/min, depth of cut 1mm and nose radius 0.8mm. The optimized parameters for cutting force obtained are also the same as that of surface roughness.From the figure 11.2the optimized parameters for minimum cutting force are obtained and are cutting speed 31.4m/min, feed rate 60mm/min, depth of cut 1mm and nose radius 0.8mm. The larger nose radius produces high cutting force. So, the smallest nose radius (0.8mm) is the optimized level of nose radius for cutting force.

ANALYSIS OF VARIANCE ANOVA is done to find out the significant factor on output parameters. The percentage influence of factors can be found out using ANOVA. It is performed with a confidence interval of 95%. The results of analysis are tabulated in table 12.1 and table 12.2. From the table 12.1,it is clear that feed rate is the most influencing factor on surface roughness followed by cutting speed and depth of cut. Noseradius has the least effect on surface roughness. From table 12.2,it is found that feed rate is the most influencing parameter on cutting force. Depth of cut and nose radius are the other important parameters that affect cutting force.The effect of cutting speed on cutting force is very less.

Impact Factor(JCC): 1.9586- This article can be downloaded from www.impactjournals.us

38

Amal T. S, Vidya V & Abraham K Varughese

Table 12.1: Anovafor Surface Roughness Source Cutting speed Feed rate Depth of cut Nose radius Error Total

DOF 2 2 2 2 0 8

SS 27.9396 87.2217 6.8012 5.3644 0.00000 127.3269

MS 13.9698 43.6108 3.4006 2.6822

F 13.9698 43.6108 3.4006 2.6822

%C 21.94 68.50 5.34 4.22

63.6634

100

Table 12.2: ANOVA for Cutting Force Source Cutting speed Feed rate Depth of cut Nose radius Error Total

DOF 2 2 2 2 0 8

SS 0.5286 4.7786 3.4565 2.4015 0.0000 11.1652

MS 0.2643 2.3893 1.7282 1.2007

F 0.2643 2.3893 1.7282 1.2007

%C 4.74 42.80 30.95 21.51

5.5825

100

The multiple linear regression model for surface roughness and cutting force are obtained and are shown in equation 3 and 4 respectively. Ra = 0.026 - 0.00761Vc + 0.002923 f + 0.096ap – 0.119rƐ F =241-2.61Vc + 0.898 f + 96.2 ap+100 rƐ

(3) (4)

Two confirmation experiments for surface roughness and cutting force are performed and the roughness value obtained is 0.2036µmand the cutting force obtained is 414.0475 N and are in in good agreement with the predicted values of regression models.

CONCLUSIONS Analysis and optimization in end milling of Ti6Al4V is done by considering four machining parameters such as cutting speed, feed rate, depth of cut and nose radius. Taguchi method and ANOVA are used to find out the optimum combination of machining parameters to minimize surface roughness and cutting force. From this study, it can be concluded that; •

The most influencing parameter on surface roughness is feed rate, which is followed by cutting speed, depth of cut and nose radius.

•

Feed rate is the most influencing parameter on cutting force, followed by depth of cut, nose radius and cutting speed.

•

The smaller nose radius produces less cutting force.

•

The optimal parameters for end milling of Ti6Al4V to reduce surface roughness (cutting speed =31.4m/min, feed rate =60mm/min, depth of cut =1mm, nose radius= 0.8mm) and the optimal parameters to reduce cutting force (cutting speed =31.4m/min, feed rate =60mm/min, depth of cut =1mm, nose radius= 0.8mm) were obtained through this study and the confirmation experiments produced low values of cutting force and surface roughness. Index Copernicus Value: 3.0 - Articles can be sent to editor@impactjournals.us

Machining Parameters Optimization in End Milling of Ti6al4v Using Taguchi Method

39

REFERENCES 1.

J.Pradeep Kumar, K.Thirumurugan, “Optimization of machining parameters for milling Titanium using Taguchi method”, IJAET, vol 3, June 2014, pp. 108-113.

2.

Rao B, Dandekar C R and Shin Y C , “An experimental and numerical study on the face milling of Ti6Al4V alloy: Tool performance and surface integrity”. Journal of material processing technology,vol 211, 2011,pp 292304.

3.

Khairi Yusuf, Y. Nukman, T. M. Yusof , S. Z. Dawal,“ Effect of cutting parameters on the surface roughness of titanium alloys using end milling process”, IJAET, June 2010, pp. 1284-1293.

4.

Lohithaksha M Maiyar, Dr.R.Ramanujam, Dr.J.Jerald,“Optimization of Machining Parameters for End Milling of Inconel 718 Super Alloy Using Taguchi Based Grey Relational Analysis”, Procedia engineering 64, 2013, pp. 1276-1282.

5.

V Krishnaraja, S Samsudeensadham, R Sindhumathi, P Kuppan, “A study on high speed end milling of titanium alloy”. Procedia Engineering 97, 2014,pp 251 – 257

6.

Nithin Tom Mathew, Gopikrishnan A., Gowrie s.“Multi objective optimization of micro turning process parameters using grey relational analysis”, Precision, meso and micro engineering, vol 1, 2013, pp. 83-89.

7.

Vijay s, Krishna raj, “Machining parameters optimization in end milling of Ti6Al4V”.procedia engineering, vol64, 2013,pp 1079-1088

8.

C.C. Tsao, “Grey-Taguchi method to optimize the milling parameters of aluminium alloy”, Int j adv manufacturing technology,vol 40,2009,pp. 41-48

Impact Factor(JCC): 1.9586- This article can be downloaded from www.impactjournals.us

5 eng machining parameters optimization amal t s

Published on Sep 18, 2015

Ti6Al4V has inevitable applications in aerospace industry where high surface finish is required. In this research the endmilling of annealed...

Advertisement